Electrical behavior and Optical Properties of Copper oxide
Issam M. Ibrahim*
Muhammad O. Salman*
Ahmed S.Ahmed *
Received 3, January, 2011 Accepted 02, May, 2011
In this work the structural, electrical and optical Properties of CuO semiconductor films had been studied, which prepared at three thickness (100, 200 and 500 nm) by spray pyrolysis method at 573K substrate temperatures on glass substrates from 0.2M CuCl2·2H2O dissolved in alcohol. Structural Properties shows that the films have only
a polycrystalline CuO phase with preferential orientation in the (111) direction, the dc conductivity shows that all films have two activation energies, Ea1 (0.45-0.66 eV) and
Ea2 (0.055-.0185 eV), CuO films have CBH (Correlated Barrier Hopping) mechanism
for ac-conductivity. The energy gap between (1.5-1.85 eV).
Key words:TCO materials;Electrical properties;Optical properties;CuO
CuO is attractive as a selective solar absorber since it has high solar absorbency and a low thermal emittance .Copper forms two well known oxides: cuprite (Cu2O) and
tenorite (CuO) . The two oxides can coexist with copper, annealing Cu2O
films in air at 300oC converts it to CuO .While Cu2O forms a cubic structure
with a lattice parameter of 4.27 Å, CuO is unique as it has a square planar coordination of copper by oxygen in the monoclinic structure. The lattice parameters of CuO are a = 4.684 Å, b = 3.425 Å, c = 5.129 Å and b = 99.28° . And its suitable optical Properties, Its band gap is reported to be between 1.3 and 1.7 eV with a black color and a partial transparency in the visible range . Due to the existence of copper vacancies in the structure, CuO exhibits native p-type conductivity . Various techniques have been used to synthesize CuO films. Low temperature deposition methods for thin film photovoltaic devices are of
interest to enable the use of lightweight, flexible substrates. Such devices provide a higher power-to-weight ratio and significant cost savings compared to current technologies . The spray pyrolysis method is a well-known thin-film preparation method with excellent features such as the need for no sophisticated equipment, and quality targets or substrates; also, film thickness and stoichiometry are easy to control and the resulting films are well compacted. We have used this coating method to prepare thin films of CuO. Table (1) below shows some of physical properties of Cu, CuO and CuCl2.2H2O..The aim of this work
Table(1) Mol. weight, physical form, density and qualitative solubility of Cu, CuO and CuCl2 ·2H2O 
Physical form Density g/ cm3 Qualitative solubility
Copper Cu 63.546 red metal- cubic 8.96 slightly soluble in dilute acid Copper(II) oxide CuO 79.545 black powder or
monoclinic crystal 6.31
insoluble in H2O, ethanol; soluble
dilute acid Copper(II) chloride dihydrate CuCl2 ·2H2O 170.482 green-blue orthorhombic crystal; hygroscopic 2.51
Very soluble in ethanol, methanol; soluble in acetone; insoluble in
Materail and Methods:
CuO films have been produced by spraying the aqueous solution of 0.2M of CuCl2 .2H2O onto the microscope
glass substrates (1x25x75mm3) at substrate temperature of 573K. The substrate temperature was maintained within ±10K. 50 ml alcohol was used for preparing the solutions.
The used CuCl2 .2H2O weight was
calculated using the following equation:
Weight (g) =Molarity (mol/l) *Volume
Prior to deposition, the substrates were cleaned with cleaner solution, distilled water and followed by alcohol using ultrasonic bath.
The schematic arrangement of spray pyrolyses set-up is shown in Fig. (1). Spray pyrolysis is basically a chemical process, that is the spraying of the solution onto a substrate held at high temperature, where the solution reacts forming the desired film.
Fig. (1) Schematic of the spray pyrolysis system.
The spray rate of the solution was adjusted to be five sprinkling in minute, the sprinkling time about ten second. The normalized distance between the spray nozzle and the substrate is 29cm. Oxygen was used as the carrier gas. The temperature of the substrate was controlled by an Iron-Constantan thermocouple. The thickness of the films (t) was determined using the weighing-method.
Where m= the mass difference of
slide after and before the deposition, A=area =2.5 7.5 cm2 and ρ= CuO mass density=6.31 g/cm3.
Crystal structure were investigated by means of a X-ray diffraction XRD Shimadzu 6000 Japan using CuKα1,
parameters were measured directly from above setup total resistance (R), total capacitance (C) and dissipation factor (tanδ) with accuracy of 0.1%. All measurements were performed under certain frequency 102 -105 Hz. The temperature range between (303- 413K) and constant voltage of (0.08 V) was applied in all frequency range and temperature those are indicated in this work.
The absorbance and the transmittance have been measured for the scanning of electromagnetic spectrum from the range (300-900nm) by the UV visible Philips (Pu 8800 – UV/VIS) spectrophotometer, to calculate from these measurements the energy gap and the other optical constants
Results and Discussions:
Fig. (2) Shows XRD for 100,200 and 500 nm thin films deposited on glass from 0.2 M CuCl2:2H2O. Three peaks
can see for (CuO) phase located at 2θ=32.49o
, 35.53oand 38.74o with hkl (110) , ( and (111) respectively. The increasing of the thickness approach the structure of the prepared films from the bulk material indicating from increasing of the grain size since the later parameter is inversely proportional with the full width maximum(FWM).
Fig (2) XRD for 100 ,200and 500 nm CuO deposited on glass
Table (2) shows the experimental peaks, observe from XRD, and the standard peaks from International
centre for diffraction data (JCPDS) for CuO film and their intensities , it shows a perfect identicalness between them.
Table (2) the experimental and the standard peaks from (JCPDS) for CuO film 2θ exp. dhkl Exp.( Å) Int. % dhkl Std.( Å) Int. % hkl 32.49o 2.753 49 2.751 12 (110) 35.53o 2.524 100 2.523 100 ( 38.74o 2.322 53 2.323 96 (111) 48.76o 1.866 24 1.866 25
The d.c. conductivity for the films has been studied as a function of temperature at different thicknesses (100, 200 and 500 nm) within the range of (303-508 K) at steep of (10 K) shown in Fig.(3).
D.c conductivity (σ ) of samples obtained using equation (3).
where L: distance separated the electrodes, R: Resistance of film, t: film thickness, d: electrodes width.
Fig.(3) The relation between Ln(σ) versus reciprocal of temperature for different film thicknesses (100, 200 and 500nm)
As seen from Fig.(3) function of ln(σ) versus reciprocal temperature, this figure declared that in all samples there are two stages of conductivity throughout the heating temperature range. The first activation energy (Ea1)
activation energy is due to conduction of the carrier excited into the extended states beyond the mobility edge, while the second activation energy (Ea2)
occurs at low temperature and the conduction mechanism of this stage is due to carriers transport to localized states near the valence and conduction bands. Also we can see the increasing of (σ) with the increasing of film thickness, this is may be because of increasing the defect states with the increasing the thickness, this is may be attributed to none uniformity in the depth composition.
Table (3) shows the d.c conductivity, Ea1 and Ea2 for different film thickness.
We can notice from this table the activation energy increase with decreasing thickness because the size of the grain decreases with increase the film thickness and that responsible for increase the mean free path of electrons and that lead to increase the conductivity.
Table (3) d.c conductivity at R.T, Ea1
and Ea2 for different film thicknesses
Thickness (nm) σ R.T (Ω.cm) -1 Activation energy (eV) Rang e (K) 100 5.48*10-6 Ea1 0.663 473-508 Ea2 0.185 303-473 200 3.66*10-4 Ea1 0.470 473-508 Ea2 0.059 303-473 500 9.7*10-4 Ea1 0.453 473-508 Ea2 0.055 303-473
A frequency dependence on a.c conductivity σa.c.(ω) has been observed
in many semiconductors to have the form :
σa.c.(ω) =A ωS ……….4
Where s is the exponent factor
Fig (4) The relation between Ln(σa.c)
and Ln ω for different temperature.
Fig. (5) Shows the variation of ac conductivity (w) as a function of frequency at different temperatures. The conductivity (w) for all samples increases as frequency becomes greater than 400Hz.In this case the conductivity is proportional to
which means that ac-conductivity dominates at higher frequencies in the range(400Hz-100KHz).For a lower frequencies in the range lower than 400Hz becomes less dependent with frequency, and it is difficult to measure the ac-conductivity component, we found that the value of (s) is between (0.14-0.30)when the temperature increases from 303K to 423K.In general, our samples have large values of the exponent(s) and it is fit with CBH model given by Long from which ac conduction occurs between two sites over the barrier separating between them as D+D- defect center in the band gap.
Fig. (6) Illustrates the dielectric loss. In practice, it is convenient to specify the absorption losses in dielectric at a given frequency and temperature by the loss tangent (tanδ ), where δ is the angle between the displacement current and its loss components 
Fig (6) The variation of dissipation factor with Lnω for different temperature.
Fig (7) shows Cole- Cole diagram for CuO films. From this figure we see that the dielectric constant increases with increasing temperatures [see table 4]. To find out the causes of dielectric dispersion such as Debye dispersion; Debye noted that insulating material is usually used over the wide range of frequency and predicated that, when an external alternating field is applied at very high frequencies, the molecular dipoles do not have enough time to change their orientation in keeping with the applied field, since its period necessary to orientate is less than the relaxation time and the dielectric comprises only the contribution from the electronic and ionic polarization. The existent dielectric constant is called optical dielectric constant
Instead at very low frequencies, the period of applied field is very large in comparison with τ, the polarization goes to its maximum value, the dielectric constants contain the full contribution from the dipoles
polarization and the power loss is zero . Here dielectric constant is called the static dielectric constant
When an external field E is applied through dielectric material, the dipoles do not attain its orientation immediately. Also the dipoles polarization requires an amount of time after removal of the external field .
Fig.(7) Cole-Cole diagram at different temperature for.
Table (4) exponent factor, polarizibility, εs and ε∞ at different
temperatures. T (K) S factor θ (deg.) α=2θ/π P(V/cm) εs ε∞ 303 0.301 5 0.055 222.22 310 20 333 0.365 3.9 0.043 173.33 620 24 353 0.235 2.25 0.025 100.00 800 25 373 0.193 0.28 0.003 124.4 910 27 393 0.191 0.24 0.0026 1.066 1040 25 413 0.149 0.21 0.0023 0.933 1200 27
From our data, we conclude that σac
(ω) is a function of the temperature of measurements. The values of ac. activation energy Eω for CuO films at
(200,1000,4000,20000,40000 and 100000 Hz) are determined from a plot of ln(σac (ω)) against the reciprocal
absolute temperature, as shown in Fig.(8).the temperature dependence of σac is logarithmic relation. We can see
that there is a weak temperature dependence of σac with increasing
frequencies in the range (303-413K).[see table 5].
Fig.(8) The relation between Ln(σA.C(ω)) versus reciprocal of T
Table (5) A.c activation energy and temperature range for different film thicknesses F (Hz) 200 1000 4000 20000 40000 100000 Eω(eV) 0.217 0.202 0.135 0.091 0.075 0.064 T Range (K) 333-413 333-413 333-413 333-413 333-413 333-413
Optical study of CuO film is carried out in the wavelength range 200–900 nm at room temperature for the film deposited on glass substrate. Figure (9) shows the room-temperature transmission spectra of three samples at different thicknesses (100, 200 and 500 nm).
Fig.(9) the transmission variation with the wave length for CuO at different thicknesses
The dependence of the absorption coefficient on the wavelength for different film thicknesses of deposited CuO films on glass is shown in Fig. (10). One can see from this figure that the absorption coefficient of the CuO films is characterized by a strong absorption at the shorter wavelength region which means that there is a
large probability of the allowed direct transition and without sharp edge on the long wavelength side from 350– 900 nm.
Fig. (10) the variation of absorption coefficient with the wave length for CuO at different thicknesses
The optical energy gap values (Egopt)
for CuOfilms have been determined by using Tauc equation. This is used to find the type of the optical transition by plotting the relations (αhυ)1/2,(αhυ)1/3,(αhυ)2/3,and (αhυ)2
versus photon energy (hυ).This equation also selects the optimum linear part. It is found that the relation for r=1/2 yields linear dependence, which describes the allowed direct transition. Egopt is then determined by
the extrapolation of the portion at (α =0 as shown in Figure 11), where the values of energy band gap are equal to 220.127.116.11 and 1.9eV for t=100,200 and 500nm respectively.
CuO films was fabricated by
chemical spray pyrolysis,with different thickness.The XRD analysis shows that the films were a polycrystalline structure.From dc conductivity invistigation we found that the process of conductivity occurs in two stages of conductivity.It has shown that from ac conductivity the exponent (s) is temperature dependent [e.g. for t=100nm thickness) which found that the value of s decreases from (0.30 to 0.14), when the temperature increases from 303K to 413K], and the conductivity exponentioally dependent on temperature.CBH is most suitable to interpret our results.the optical energy gap indicates not systematic behaviur with increasing thicknesses.
 Yoon K H, Choi W J and Kang D H.2000. Photo electrochemical properties of copper oxide thin films coated on an n-Si substrate, Thin Solid Films 372: 250.
 Richthofen A, Domnic R, Cremer R and Fresenius J.1997 .Preparation of cuprite (Cu2O),
paramelaconite (Cu32+Cu21+O4) and tenorite (CuO) with magnetron sputtering ion plating, J.Anal. Chem. 358: 312-317.
 Pathan H. M. and Lokhande C. D.2004. Deposition of Metal Chalcogenide Thin Films by Successive Ionic layer Adsorption and Reaction (SILAR) method, Bull. Mater. Sci.27 (2):85-92.
 David R. Lide 2006.CRC Handbook of Chemistry and Physics, ed. Taylor and Francis, Boca Raton, FL,.
 Ohya Y, Ito S, Ban T and Takahashi Y.2000.Preparation of CuO thin films and their electrical conductivity, Eng. Mater 181:113-116.
 Jeong Y K and Choi G M.1996. Nonstoichiometry and electrical conduction of CuO, Phys. Chem. Solids 57:81-86.
 Zhang, L., Yu, J. C., Xu A. W., Li Q., Kwong, K. W., Yu S. H. 2004.Peanut-shaped nanoribbon bundle superstructures of malachite and copper oxide, J.Cryst. Growth 266: 545-550.
 Cruz M., Herna´L.n, Morales J., Sa´nchez L.2002. Spray pyrolysis as a method for preparing PbO coatings amenable to use in lead-acid batteries" Power Sources108:35-41.
 JCPDS Data Base, Card No. 05-0661.
 Jonscher A. K.1976. Alternating current diagnostics of poorly conducting thin films, Thin Solid Film, 36: 1-20.
 Davis E.A., Mott N. F.1979. Electronic processes in non-crystalline materials, Clarodon Press, Oxford : 223.
 Scaife B. K. 1989. Principle of dielectrics, Clarendon press, Oxford.600.